Macromolecules 2010, 43, 5804–5813 DOI: 10.1021/ma100841c
Micrometer and Submicrometer Particles Prepared by Precipitation Polymerization: Thermodynamic Model and Experimental Evidence of the Relation between Flory’s Parameter and Particle Size Antonio L. Medina-Castillo,* Jorge F. Fernandez-Sanchez,* Antonio Segura-Carretero, and Alberto Fernandez-Gutierrez Department of Analytical Chemistry, University of Granada, Avd. Fuentenueva s/n, 18071 Granada, Spain Received April 16, 2010; Revised Manuscript Received May 31, 2010
ABSTRACT: This work highlights the relevance of the interactions between polymer and solvent during precipitation polymerization in order to control the morphology and the size of the precipitated material without any changes in chemical composition. Thus, a thermodynamic model based on Flory Hugings model and Hansen’s solubility parameters has been proposed in order to control the precipitation process. This model is based on the study and characterization of the interactions (hydrogen-bonding forces, polar forces and dispersion forces) between growing polymeric chains and solvent molecules. The model was corroborated by more than 80 different solvent compositions were used for a ternary solvent mixture (toluene, acetonitrile and 2-propanol) and two different monomer molar ratio feeds (45% MAA, 20% HEMA, and 35% EDMA; 20% MAA, 45% HEMA, and 35% EDMA). The morphologies of the resulting polymer material were characterized by scanning electron microscopy and transmission electron microscopy and the particles sizes were deduced by dynamic light scattering. The polymeric particles with different sizes prepared in this work were used to introduce on them magnetic properties. The results in this work enable the control of the size, chemical composition, and the homogeneous encapsulation of Fe3O4 within different hydrophilic polymeric matrixes by polymerization precipitation, allowing the design of magnetic particles free of any stabilizers.
1. Introduction Copolymer microspheres are attractive for many applications, due to their unique morphology and designed surface properties. For instance, uses as adsorbents, stationary phases for chromatography, supports for exchange, membrane materials, catalysis, sensors, and carriers as well as supports in biomedical and environmental fields, are possible due to their unique morphology and designed surface properties.1-5 Therefore, the control of the surface properties of particles is key in many areas and in numerous commercial technologies, ranging from biotechnology to advanced microelectronics.6,7 Emulsion, suspension, and dispersion polymerization are wellknown techniques for preparing copolymer microspheres and nanospheres. However, it is often tedious to remove the surfactant or stabilizer necessary for stabilizing of the microspheres during their preparation. Precipitation polymerization is unique to prepare polymeric microspheres of uniform size and shape free of any added surfactant or stabilizer. This technique starts as a homogeneous mixture of monomer, initiator, and optional solvents, and during the polymerization, the growing polymeric chains are separated from the continuous medium by changes in the mixing free energy.8 In recent years, precipitation polymerization has been widely used to prepare narrow or monodispersed microspheres with different functional chemical groups on their surfaces, in the absence of any stabilizer or additive, and without stirring. The control of *Corresponding authors. (A.L.M.C.) Telephone: þ34 958248593. Fax: þ34 958249510. E-mail: [email protected]
(J.F.F.-S.) Telephone: þ34 958248409. Fax: þ34 958249510. E-mail: [email protected]
Published on Web 06/10/2010
the size and the uniformity of the resulting polymeric particles has been major area of interest, especially for particles in the micrometer and submicrometer size range. A main disadvantage is the difficulty in obtaining monodispersed hydrophilic polymeric microspheres with good spherical shape by this polymerization technique.9 Several experiments have been carried out to establish the effect of the initial molar monomers (which contain hydroxyl and acid groups such as MAA and HEMA) ratio feed on the morphology and size of microspheres produced by precipitation polymerization in nonpolar solvents.10-12 Less attention has been paid to the effects of the microspheres on the morphology and size by the changes caused in the interactions between polymeric growing chains and solvent molecules when the initial molar monomers ratio feed is kept constant.In addition, the previously reported data are rather qualitative since they may require tedious theoretical thermodynamic treatments. This paper describes a thermodynamic model based on the Flory-Huggins model and Hansen solubility parameters, allowing us to delve into knowledge of the precipitation process in precipitation polymerization. This model is based on the study and characterization of the interactions (hydrogen bonding and polar and dispersion forces) between growing polymeric chains and solvent molecules, because change in these interactions provides the desolvation and collapse of the network at different growth levels. This phenomenon is analogous to the cloud point observed when a solution containing one homopolymer is heated above the lower critical solution temperature (LCST).10 Correlations between the morphology of the polymeric network (soluble copolymer, macrogels, gels, and spherical colloids) with the polymer-solvent interactions will be given in order to r 2010 American Chemical Society
Macromolecules, Vol. 43, No. 13, 2010
show the versatility of the model. In addition, this model can be used to correlate the particle size of spherical colloids with the polymer-solvent interactions. Therefore, the model allows micrometer and submicrometer particles of different sizes to be synthesized without changing the molar monomer ratio feed. Finally, hydrophilic magnetic micrometer and submicrometer particles were synthesized by precipitation polymerization.
On the other hand, it is possible to correlate the Flory’s parameter with Hansen’s solubility parameters. Hansen divided the solubility parameters into contributions for dispersion (δd), dipole (δp), and hydrogen-bonding (δh) interactions.19 It is possible to express the solubility parameters for a mixture of i solvents as δi, j ¼
φi δi, j ;
j ¼ d, p, h
2a. Flory-Huggins Model and Hansen Solubility Parameters. According to the Flory-Huggins theory for polymer solutions, the free energy of a mixture is:13-15
where δhj is the j solubility parameter of the mixture, Φi is the volume fraction of solvent i and δi,j is the solubility parameter j of solvent i.20 This expression may be applied for an ideal mixture of solvents with similar molar volumes. The solubility parameter model has been successful in describing thermodynamic properties of polymer solutions. It shows that the Flory’s parameter can be related to the three-dimensional solubility parameters21,22 by Vs χs, p ¼ ð9Þ R s, p 2 RT
The subscripts s and p are the corresponding labels for solvent and polymer, respectively, χp,s is the Flory’s parameter which is related with the interaction between solvent molecules and polymer segments, Φ is the volume fraction, and the parameter x is often interpreted as the number of lattice segments occupied by a given polymer and it is estimated as the volume molar ratio of polymer and solvent.13-16 The volume fraction of the polymer can be expressed as
where Vs is the molar volume of the solvent when using one solvent or an average molar volume in solvent mixtures,18,22 and Rs,p2 is a modified difference between the Hansen solubility parameter for a solvent (s) and a polymer (p). A useful concept that quantifies the similarity of polymer, p, and solvent, s, is the solubility parameter distance (Rs,p),22 defined by
ΔGmix ¼ ns RTχs, p Φp þ RT½ns ln Φs þ np ln Φp
where enthalpic and entropic contributions are given by: ΔHmix ¼ ns RTχs, p Φp ,
ΔSmix ¼ RT½ns ln Φs þ np ln Φp
where Np is the number of polymer molecules and N0 is the total numbers of molecules (solvent and polymer). For diluted polymer solutions, small changes in the polymer molecular weight (x) do not result in large increases of Φp (see eq 3). In addition, the Flory parameter χs,p is related to the coordination number of the lattice (z) and the interchange energy (Δw) by the following expression:17 χ s, p ¼ -
Here the interchange energy, Δw, is the energy difference involved in breaking a solvent-solvent interaction (wss) and a polymer-segment-polymer-segment interaction (wpp) to form two solvent-polymer-segment interactions (wsp): Δw ¼ ðwss þ wpp Þ - 2wsp
Also, Δw can be interpreted as an free-energy exchange with enthalpic and entropic contributions:17 ΔwG ¼ ΔwH - TΔwS
zΔwH zΔwS þ χs, p ¼ χs, p, H þ χs, p, S ¼ 2RT 2R
In addition, χs,p is related with the polymer size, i.e., with the average molecular weight of a polymer; an increase in the average molecular weight provides an increase of the χs,p. This has been experimentally demonstrated,17,18 but there is not any theoretical relation between molecular weight and Flory’s parameter.
Rs, p ¼ ½4ðδd , p - δd , s Þ2 þ ðδp, p - δp, s Þ2 þ ðδh, p - δh, s Þ2 1=2 ð10Þ This means that the polymer solvent interactions increase when the solubility parameter distances decrease. When χs,p is less than 0.5, the solvent is generally classified as a good solvent for the polymer, while a value higher than 0.5 is a poor solvent and may lead to phase separation.23 It can be applied in mixtures of the two and three noninteracting solvent systems.9,18,22-26 The three-dimensional Hansen’s solubility parameters can be simplified into a dimensional one.27 Therefore, threedimensional coordinates (δp, δd and δh) are converted into two-dimensional coordinates (PDs,p and Hs,p). The relation between PDs,p and Hs,p parameters with δp, δd and δh is PDs, p 2 ¼ 4ðδd , s - δd , p Þ2 þ ðδp, s - δp, p Þ2
Hs, p 2 ¼ ðδh, s - δh, p Þ2
where the subscripts s and p denote the solvent mixture and polymer, respectively. Thus, PDs,p can be used to characterize dispersion and polar interactions between the polymeric growing chains and solvent, and Hs,p the hydrogen bonding interactions between the polymeric growing chains and solvent. With eqs 10, 11, and 12, the solubility parameter distance (Rs,p) can be rewritten as Rs, p ¼ ðPDs, p 2 þHs, p 2 Þ1=2
2b. Precipitation Mechanism. It is well-known that the particle formation by polymerization precipitation consists with two stages: nucleation and growth.28 Therefore, the
Macromolecules, Vol. 43, No. 13, 2010
Figure 1. Different steps for the formation of different polymeric network morphologies by precipitation polymerization. Key: radical initiator (I), monomer (M), and polymeric growing chains (MNþ1, Mnþ1; N and n indicate the average number of monomers forming the polymeric chain, N > n).
system is homogeneous prior precipitation and, as soon as the polymerization starts, primary radicals, generated by decomposition of the initiator, grow by the addition of monomer units and provide solvated polymeric growing chains (monophasic system). This occurs until the systems reach to their maximum molecular weight, which can be solvated by the media. At this moment, when the media cannot solvate the polymeric growing chains, the separate-phase and precipitation process starts, and N polymeric growing chains interact spontaneously with each other to produce the precipitation28 (see Figure 1, step a) thus the transparent and homogeneous reaction mixture becomes a milky white dispersion. Finally, the particle growing step can happen in two ways:29 1) by capturing oligomer radical and monomer on the particle surface (see Figure 1, step b), or 2) by aggregation of nuclei to form the mature particles by a homocoagulation process (see Figure 1, step c). If the solvent medium is suitable, the polymeric chains grow too much and they precipitate as a gel (see Figure 1, step d). 3. Experimental Section 3a. Experimental Conditions Used for Precipitation Polymerization. In this work, all the experiments were performed without stirring, maintaining constant molar monomers and crosslinked ratio feed, using diluted concentrations of monomers (2.5% w/v), a pressure of 1 atm, a temperature of 82 °C, a reaction time of 1.30 h, and a total volume of solvent media of 16 mL. The conditions for selecting solvents, monomers, and radical initiator were as follows: (a) The solvents should be selected to provide an ideal mixture, or at least as ideal as possible.24,32 (b) The monomers should be compatible; hence the reactivity ratio between the monomers and cross-linker is related to the formation of a statistical polymer during the polymerization reaction. (c) Monomers and solvents must be miscible with respect to each other, and the radical initiator must be soluble in this monomer-solvent mixture. With these conditions, the solvents selected were: toluene, acetonitrile, and 2-propanol; the monomers were hydroxyethyl
Medina-Castillo et al. methacrylate (HEMA) and methacrylic acid (MAA); the crosslinker was ethylenglycol dimethacrylate (EDMA); and the radical initiator was azobis(isobutyronitrile) (AIBN). In this work, two different molar monomer ratio feeds were used (45% MAA-20%HEMA-35%EDMA, called P1, and 20%MAA45%HEMA-35%EDMA, called P2). 3b. Magnetic Hybrid Nanoparticles Encapsulated by EDMA/ MMA/HEMA (EDMA/MMA/HEMA-Fe3O4-OA). Magnetite coated with oleic acid (lipophilic magnetic nanoparticles) was prepared by the conventional method.31 Then, 2 g of lipophilic magnetic nanoparticles were dispersed in 5 mL of n-heptane and added to 400 mL of Milli-Q water containing 250 mg of SDS. The ice-cooled mixture was sonicated for 20 min in a high-energy sonifier (BRANSON, S-450D) at 70% amplitude for 20 min. The resulting mini-emulsion was transferred slowly (under mechanical stirring) to a double-necked flask containing 1.5 mL of 26 wt % MMA, 60 wt % EDMA, and 14 wt % HEMA. The mixture was stirred for 2 h at room temperature. Next, 180 mg of potassium peroxodisulfate (KPS) was added to start the polymerization, and the reaction system was heated to 65 °C under a gentle stream of nitrogen. After a polymerization time of 24 h, the resulting product was washed six times with Milli-Q water, five times with acetone, and five times with methanol in order to eliminate surfactant and unreacted compounds. 3c. Magnetic Particles Containing EDMA/MMA/HEMAFe3O4-OA Prepared by Precipitation Polymerization. The experimental conditions to prepare magnetic particles by precipitation polymerization were selected taking into account the results found in the control of particle size for systems P1 and P2. Two different conditions were selected: (1) the experimental conditions to obtain 1100 nm particles of P1 and (2) the experimental conditions to obtain gels for P1 and P2 systems. Precipitation polymerizations were developed in the presence of 5 wt % (with respect to the monomer mixture) of the EDMA/ MMA/HEMA-Fe3O4-OA nanoparticles prepared in section 3b following the protocol described in section 3a. 3d. Morphological Characterization. The particles prepared in this work were washed with methanol several times and then the particle size was measured in methanol by dynamic light scattering (Zetasizer Nano ZS-90, Malvern Instrument). The morphology of the materials prepared in this work was analyzed by scanning electron microscopy (SEM) and high resolution transmission electron microscopy (HRTEM).
4. Results and Discussion 4a. Assumptions To Model the Precipitation and Formation of Different Polymeric Network Morphologies. Under the experimental conditions mentioned above and making an appropriate selection of solvents (ideal mixture) and monomers for the formation of the statistical polymer (see section 3a), we propose the following assumptions: (a) The polymeric chains grow solvated by the media (ΔGmix 0. Therefore, ΔSprec and ΔHprec must be negative and therefore we can conclude that precipitation occurs when jΔHprec j > TjΔSprec j
Before precipitation, the polymeric growing chains are solvated (monophasic system); this means that ΔGprec is positive and ΔGmix is negative.21 Then, these chains continue growing and their average molecular weight is increased. As commented before, an increase in the average molecular weight increases Flory’s parameter and hence increases Rs,p (see eq 9). The free energy of a mixing can be related with the Flory’s parameter (see eq 1).18,30 Thus, greater molecular weight results in an increase in the ΔHmix and therefore of ΔGmix (see eqs 1 and 2). Therefore, sometime during the polymerization reaction, the value of ΔGmix = 0. We define this moment as the inflection or critical point (I.C.). At this point, under the experimental condition mentioned above, the Flory’s parameter at the I.C. point (χs,p,IC) can be calculated by eq 9. For this we have to consider assumption b (see section 3a), which allows the calculation of the minimum statistical polymer unit and therefore the value of its Hansen solubility parameter, and the Hansen solubility parameters of the solvent mixture at I.C. point. With assumptions d and e (see section 4a), it is possible to establish a relationship between average molecular weight of the polymeric growing chains and particle size. Bearing in mind that average molecular weight can be related with the Flory’s parameter, we can say that particle size ¼ f ðχs, p, IC Þ
We will demonstrate that for evaporation lower than 20% of the initial volume of solvent mixture, the composition of the solvent mixtures is practically constant before precipitation. Thus, Flory’s parameter at the IC point (χs,p,IC) can be approximated to the initial Flory’s parameter (χs,p,0), and eq 15 can be rewritten as follows: particle size ¼ f ðχs, p, 0 Þ
This consideration will be demonstrated experimentally in section 4c. In addition, we will demonstrate that it is possible to control the particle size in a wide range by changing the
Figure 2. Qualitative thermodynamic diagrams to analyze the different polymeric network morphologies versus χs,p and the shape of the variation of ΔGprec during the polymerization for the formation of a statistical copolymer in ideal mixtures of solvents. One (gray lines) corresponds with solvated copolymers; 2 (thin short-dash black line) correspond with a gel; 3 and 4 (bold black line) correspond with spherical particles of different size (the size of 3 is higher than the size of 4); 5 (bold dash line) corresponds with a nonspherical particle formed by homocoagulation process.
solvent media without changing the molar ratio of monomers and cross-linked feed. To continue with the polymerization process, after I.C. point, the phase separation and precipitation process starts. Separate-phase and precipitation process will continue until the ΔGprec rises to a minimum value. The polymeric network morphologies can be related with the value of the Flory’s parameter at the I.C. point, and the number of times that ΔGprec reaches a minimum value after arriving at the I.C. point (see Figure 2). A small value of Flory’s parameter at the I.C. point means that the average molecular weight of the polymeric growing chains is high, so that, after the I.C. point they should precipitate by forming an amorphous material (gel). Otherwise, a high value of Flory’s parameter at I.C. point means that the average molecular weight of the polymeric growing chains just before precipitation is short, so their precipitation provides particulate materials. This approach will be confirmed by experimental data in section 4e. Also, the ranges of Flory’s parameter in which the different materials are obtained will be determined in section 4f. The particulate material can be spherical particles or nonspherical particles formed by a homocoagulation process. This depends of the numbers of times that ΔGprec reaches a minimum value after the I.C. point. If ΔGprec reaches only a minimum value once, narrow disperse spherical particles result. If ΔGprec reaches to a minimum value twice, spherical particles are produced first, and then coagulation processes between particles occur, giving rise to nonspherical particles formed by the homocoagulation process (see Figure 2). 4c. Relationship between Initial and I.C. Point Flory’s Parameters. In this section, we will demonstrate that eq 15 can be rewritten as eq 16, and therefore χs,p,IC ≈ χs,p,0. If the composition of the solvent mixture changes by evaporation, Flory’s parameter also changes during polymerization. To analyze the effect of solvent evaporation on the Flory’s parameter, we evaluated four solvent compositions. The first is based on a unique solvent (acetonitrile), and thus the Flory’s parameter is not affected by evaporation. The molar fraction of each solvent in the other three compositions were as follows: composition 2, XToluene=0.5, XAcetonitrile= 0.25, X2-Propanol = 0.25; composition 3, XToluene= 0.6, XAcetonitrile= 0.25, X2-Propanol= 0.15; composition 4, XToluene= 0.3, XAcetonitrile= 0.35, X2-propanol= 0.35). The monomer feed molar percentage was 45% MAA, 20% HEMA and 35% EDMA (P1 system, see section 3a).
Macromolecules, Vol. 43, No. 13, 2010
Medina-Castillo et al. Table 1. Group Increments for Calculating the Solubility Parameters of Statistical Polymeric Minimum Units in P1 and P2 Systems18 Fpi Fdi Vi Ehi (J mol-1) (J1/2 cm3/2 mol-1) (J1/2 cm3/2 mol-1) (cm3 mol-1) -COOH -OH -COO-CH3 -CH2>CH>C